• Views 1,076
• Citations 1
• ePub 42
• PDF 708
`Journal of CeramicsVolume 2013 (2013), Article ID 261914, 6 pageshttp://dx.doi.org/10.1155/2013/261914`
Research Article

## Effect of Processing on Synthesis and Dielectric Behavior of Bismuth Sodium Titanate Ceramics

1Department of Physics and Material Science & Engineering, Jaypee Institute of Information Technology, Noida 201307, India
2Electroceramics Group, Solid State Physics Laboratory, Defence Research and Development Organization (DRDO), Timarpur, Delhi 110054, India

Received 29 June 2012; Accepted 20 November 2012

Copyright © 2013 Vijayeta Pal et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

#### Abstract

An effort has been made to synthesize polycrystalline (abbreviated as BLNT) system with compositions x = 0, 0.02, and 0.04 by novel semiwet technique. Preparation of A-site oxides of BLNT for composition x = 0 was optimized using two precursor solutions such as ethylene glycol and citric acid. The XRD patterns revealed that the sample prepared by ethylene glycol precursor solution has single phase perovskite structure with a rhombohedral symmetry at RT as compared to the sample prepared by citric acid. Ethylene glycol precursor has been found to play a significant role in the crystallization, phase transitions, and electrical properties. The studies on structure, phase transitions, and dielectric properties for all the samples have been carried out over the temperature range from RT to 450°C at 100 kHz frequency. It has been observed that two phase transitions (i) ferroelectric to antiferroelectric and (ii) antiferroelectric to paraelectric occur in all the samples. All samples exhibit a modified Curie-Weiss law above Tc. A linear fitting of the modified Curie-Weiss law to the experimental data shows diffuse-type transition. The dielectric as well as ferroelectric properties of BLNT ceramics have been found to be improved with the substitution of La elements.

#### 2. Experimental Procedures

A novel semiwet technique was used to prepare lead-free ceramic (BLNT) system. These compositions were prepared using analytical-grade metal oxides or nitrate powders of sigma Aldrich as raw materials such as (99%), (99%), (99%), (99.9%) citric acid, and ethylene glycol. In this method, A-site of BLNT with composition was prepared by using two different precursor solutions; the first one is citric acid, and; the second is ethylene glycol. In the first process, an appropriate amount of citric acid solution was added to the solution of nitrates of A-site cations in a beaker (C/M ~ 1 : 1). Aqueous ammonia in the solution form was added drop by drop to adjust the pH value of the solution in the range of 6–8. The precursor solution was dehydrated by putting on heater with continuous stirring at for 3 hrs to form a viscous gel which was placed in an oven at for overnight to combust the gel into ash powder. In the second process, stoichiometry amount of the solution of nitrates of A-site cation was dissolved with the ethylene glycol (E/M  ~  1 : 1) with continuous stirring for 30 min to get homogeneously mixed solution. The precursor solution was dehydrated by the same conditions, which is discussed in the first method to form a gel into ash powder. Both precursor solutions are expected to distribute the cations atomically homogeneously throughout the polymeric structure forming a stable polymeric complex, which was combusted at appropriate temperature (°C) in the form of ash powder. The ash, highly fine, homogeneous, and highly reactive powder was mixed with appropriate amounts of powder thoroughly in ethanol using mortal pestle for 2 hrs followed by solid state route. These powders were dried and calcined at (2 hrs) for BNT-CA and BNT-EG and calcined at (2 hrs) for BLNT samples. The calcined powder was mixed thoroughly with a polyvinyl alcohol (PVA) binder solution and then pressed into the form of disk with 10 mm diameter. All samples are in pellet form, kept in alumina boat, and sintered at temperature for 2 hours. Two pellets of each composition were electroded with silver paint on both the surfaces of the samples for the subsequent electrical measurements. The crystallite size of all the samples in BLNT system was calculated using Debye-Scherrer formula () where is the average crystallite size, is the wavelength of X-ray radiation, is the full width at half maximum (FWHM), and the diffraction angle. The corresponding values are reported in Table 1.

Table 1: Dielectric properties of all BLNT system, prepared using ethylene glycol precursor.

The crystalline structure of the sintered samples was examined using X-ray diffraction (XRD) analysis with Cu-Kα radiation (DX-1000). The surface morphology of sintered ceramics was observed by scanning electron microscopy (SEM, model JEOL A 800). The dielectric constant and dielectric loss of the ceramic samples at were measured as a function of temperature over the temperature range from room temperature to using an LCR meter . A conventional P-E  loop tracer (Marine India), which is based on Sawyer-Tower circuit, was used to measure the polarization-electrical field (P-E) hysteresis loop at .

#### 3. Results and Discussion

In the present work, preparation of pure was optimized using two chemical precursors, citric acid and ethylene glycol. These samples are abbreviated as BNT-CA and BNT-EG (Figures 1(a) and 1(b)). It is observed from the XRD patterns that the sample prepared by ethylene glycol precursor solution has shown better phase formation, whereas BNT-CA has formed partially along with the presence of other phase identified as [13]. The experimental density observed in BNT-EG sample was which is 95% of theoretical density and the experimental density observed in BNT-CA sample was which is 91% of theoretical density. Therefore, a typical (BLNT) system with compositions and was prepared by semiwet technique using ethylene glycol precursor, calcined at . The XRD patterns of all the samples in BLNT system have shown single phase formation with a rhombohedral symmetry in Figure 2.

Figure 1: XRD patterns of (a) BNT-EG and (b) BNT-CA samples.
Figure 2: XRD patterns of BLNT system with compositions , and 0.04.

Pure BNT and BLNT powders have rhombohedral symmetry at room temperature. However, rhombohedral structure is hard to distinguish due to the overlapping of peaks that could be due to nearly cubic lattice parameter. Owing to small degree of rhombohedral distortion, diffraction lines were indexed on the basis of pseudocubic unit cell [14] and lattice parameters of all the BLNT samples, prepared by ethylene glycol, are calculated by using the Unit Cell program package [15]. There is a variation in the lattice parameters because of the different sizes of ionic radius of (1.03 Å) which are close to ionic radius (0.96 Å) and (0.99 Å). The values in the parentheses refer to the Shannon’s effective ionic radius with the coordination number of six taken from [16].

The microstructure of the pure BNT ceramics, prepared by semiwet using ethylene glycol and citric acid, sintered at is shown in Figure 3. Ethylene glycol precursor plays a significant role in the grain growth and densification. The microstructure of pure BNT-EG ceramics is denser, homogeneous, and uniform grains with grain size of 2.12 μm as compared to BNT-CA with grain size of 1.19 μm.

Figure 3: Microphotographs patterns of (a) BNT-EG and (b) BNT-CA samples.

The dielectric measurements of electroded samples of BNT-EG, BNT-CA, and BLNT samples were carried at frequency over temperature range from room temperature to and are shown in Figures 4(a), 4(b), 4(c), and 4(d), respectively.

Figure 4: Variations of and tan  with temperature for samples (a) BNT-EG, (b) BNT-CA, (c) BLNT with , and (d) .

Two dielectric anomalies in all the samples are shown at temperatures and , termed as “” and “” respectively, which corresponds to dielectric transitions from ferroelectric (FE) to anti-ferroelectric (AFE) and anti-ferroelectric (AFE) to paraelectric (PE), respectively. The corresponding peaks also appear in tan versus plots. However, the low value of dielectric constant of the sample, prepared using citric acid (BNT-CA), may be due to formation of other phases of , which hampers the one dielectric anomaly and relative value of dielectric constant in this sample. It has been observed that the and shift to higher temperature with increasing the concentration of . The partial replacement of A-site cation, with larger ionic radius cations and larger amount, decreases the relative displacement of B-site cation with respect to the oxygen octahedral cage and hence the increase in transition temperature is observed with substitution of La at A-site. It is obvious that (1.03 Å) can occupy the A-site of (0.96 Å) or (0.99 Å). When occupies A-site of , it will lead to charge imbalance, which creates defects on A-site. In general, A-site substitution by in BNT ceramics can be formulated in the following way: When occupies Bi-site, as shown in (1), the substitution of by may cause the slack of BLNT lattice. The lattice deformation can make the ferroelectric domains reorientation more easily. It leads to the enhancement of dielectric as well as ferroelectric properties. Additionally, can also occupy the A-site of , as shown in (2). In this case, the valence of ion is higher than that of ion. To maintain overall electrical neutrality, acts as a donor leading to some Na-site vacancies [], which can relax the strain caused by reorientation of domains. Therefore, the movement of the domains becomes easier and thus the electrical properties of the BLNT ceramics are improved significantly. Thus, the substitution of in BNT system has significantly influenced the phase transition and dielectric behavior (Figures 4(c) and 4(d)). The highest value of (~3020) and lowest value of Tan  (~0.045) are obtained with the composition in the BLNT system at room temperature. The physical and dielectric properties of all the BLNT samples are tabulated at RT in Table 1.

It shows the typical character of a ferroelectric behavior around transition temperature because of diffused phase transition. Dielectric constant exhibits strong frequency dependence above and the maximum value of decreases as frequency increases in the BNT-EG samples suggesting that the ceramic is relaxor ferroelectric. The diffuseness in the phase transition can be described by in relaxor ferroelectrics [17], where is the maximum value of dielectric constant at , is the degree of diffuseness, and is the curie-like coefficient. can have a value ranging from 1 for normal ferroelectric to 2 for an ideal relaxor ferroelectric. This sample exhibits a linear relationship. The value of the exponent “” was determined by least-squared fitting experimental data to the equation which is in the range of 1.50 to 1.80. This confirms the diffuse phase transition in BLNT-EG system. The polarization-electrical field (P-E) hysteresis loop is shown in Figures 5(a) and 5(b). It has been found that the P-E loop of BNT using citric acid is round shaped, not well developed (saturated), Figure 4(a). BNT-CA sample gets breakdown with increasing electric field. This may be due to (I) large leakage current and (II) due to insufficient annealing process. P-E loop for BNT sample prepared using ethylene glycol is well developed or saturated, Figure 5(b).

Figure 5: The P-E hysteresis loops at RT (50 Hz) (a) for BNT-CA and (b) BNT-EG.

This may be attributed to smaller grain size and relatively better density of the samples and confirm that all the samples are ferroelectric in nature.

The ferroelectric properties of all the BLNT system are tabulated at RT (50 Hz) in Table 2.

Table 2: Ferroelectric properties of all saturated BLNT system, prepared using ethylene glycol precursor.

#### 4. Conclusion

In summary, ethylene glycol prepared samples have revealed better crystallization of pure phase for BNT-EG sample. XRD patterns have revealed that the sample BNT-EG has single phase perovskite structure with a rhombohedral symmetry at RT. The structural, phase transition, and electrical properties of all the samples were investigated. The Bismuth sodium titanate, prepared by ethylene glycol precursor, has not only shown excellent dielectric but also ferroelectric behavior. The BNT sample has high value of dielectric constant (), dielectric loss , remnant polarization (μC/Cm2), and Coercive field at room temperature. The relatively highest value of dielectric constant for BLNT with composition may be attributed to the La doping. Composition with La substitution of has shown the highest value of dielectric constant and low loss as well as the highest value of remanent polarization (μC/Cm2). The transition temperature Tm is also maximum for this composition which reveals that the material can be useful for high-temperature device applications.

#### Acknowledgment

One of the authors Ms. V. Pal is thankful to JIIT for providing teaching assistance ship and other research facilities to carry out her research work at JIIT, Noida (India).

#### References

1. B. Jaffe, W. R. Cook Jr., and H. Jaffe, Piezoelectric Ceramics, vol. 3, Academic Press, London, UK, 1971.
2. M. Pecht, Y. Fukuda, and S. Rajagopal, “The impact of lead-free legislation exemptions on the electronics industry,” IEEE Transactions on Electronics Packaging Manufacturing, vol. 27, no. 4, pp. 221–232, 2004.
3. G. A. Smolenskii, V. A. Isupov, A. I. Agranovskaya, and N. N. Krainik, “New ferroelectrics of complex composition,” Soviet Physics, Solid State, vol. 2, pp. 2651–2654, 1961.
4. T. Takenaka, K. I. Maruyama, and K. Sakata, “$\left({\text{Bi}}_{1/2}{\text{Na}}_{1/2}\right){\text{TiO}}_{3}\text{-}{\text{BaTiO}}_{3}$ system for lead-free piezoelectric ceramics,” Japanese Journal of Applied Physics, Part 1, vol. 30, no. 9, pp. 2236–2239, 1991.
5. A. Sasaki, T. Chiba, Y. Mamiya, and E. Otsuki, “Dielectric and piezoelectric properties of (Bi0.5Na0.5)TiO3-(Bi0.5K0.5)TiO3 systems,” Japanese Journal of Applied Physics, Part 1, vol. 38, no. 9, pp. 5564–5567, 1999.
6. B. J. Chu, D. R. Chen, G. R. Li, and Q. R. Yin, “Electrical properties of Na1/2Bi1/2TiO3-BaTiO3 ceramics,” Journal of the European Ceramic Society, vol. 22, no. 13, pp. 2115–2121, 2002.
7. P. Pookmanee, G. Rujijanagul, S. Ananta, R. B. Heimann, and S. Phanichphant, “Effect of sintering temperature on microstructure of hydrothermally prepared bismuth sodium titanate ceramics,” Journal of the European Ceramic Society, vol. 24, no. 2, pp. 517–520, 2004.
8. Q. Xu, X. L. Chen, W. Chen, B. H. Kim, S. L. Xu, and M. Chen, “Structure and electrical properties of (Na0.5Bi0.5${\right)}_{1-\text{x}}$ Bax TiO3 ceramics made by a citrate method,” Journal of Electroceramics, vol. 21, no. 1–4, pp. 617–620, 2008.
9. D. L. West and D. A. Payne, “Preparation of 0.95Bi1/2Na1/2TiO3·0.05BaTiO3 ceramics by an aqueous citrate-gel route,” Journal of the American Ceramic Society, vol. 86, no. 1, pp. 192–194, 2003.
10. J. G. Hou, Y. F. Qu, W. B. Ma, and D. Shan, “Synthesis and piezoelectric properties of (Na0.5Bi0.5)0.94Ba0.06TiO3 ceramics prepared by sol-gel auto-combustion method,” Journal of Materials Science, vol. 42, no. 16, pp. 6787–6791, 2007.
11. J. Hao, X. Wang, R. Chen, and L. Li, “Synthesis of (Bi0.5Na0.5)TiO3 nanocrystalline powders by stearic acid gel method,” Materials Chemistry and Physics, vol. 90, no. 2-3, pp. 282–285, 2005.
12. A. P. Singh, S. K. Mishra, D. Pandey, C. D. Prasad, and R. Lal, “Low-temperature synthesis of chemically homogeneous lead zirconate titanate (PZT) powders by a semi-wet method,” Journal of Materials Science, vol. 28, no. 18, pp. 5050–5055, 1993.
13. K. Kitagawa, T. Toyoda, K. Kitagawa, and T. Yamamoto, “(Bi1/2Na1/2)TiO3 additive effect for improved piezoelectric and mechanical properties in PZT ceramics,” Journal of Materials Science, vol. 38, no. 10, pp. 2241–2245, 2003.
14. E. Fukuchi, T. Kimura, T. Tani, T. Takeuch, and Y. Saito, “Effect of potassium concentration on the grain orientation in bismuth sodium potassium titanate,” Journal of the American Ceramic Society, vol. 85, no. 6, pp. 1461–1466, 2002.
15. N. Chaiyo, A. Ruangphanit, R. Muanghlua, S. Niemcharoen, B. Boonchom, and N. Vittayakorn, “Synthesis of potassium niobate (KNbO3) nano-powder by a modified solid-state reaction,” Journal of Materials Science, vol. 46, no. 6, pp. 1585–1590, 2011.
16. R. D. Shannon, “Revised effective ionic radii and systematic studies of interatomic distances in halides and chalcogenides,” Acta Crystallographica, vol. 32, pp. 751–767, 1976.
17. K. Uchino and S. Nomura, “Critical exponents of the dielectric constants in diffused-phase-transition crystals,” Ferroelectrics Letters Section, vol. 44, no. 3, pp. 55–61, 1982.